Download presentation

Presentation is loading. Please wait.

Published byAnnika Jewison Modified over 3 years ago

1
A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State Martin Lévesque*, Katell Derrien*, Didier Baptiste* Michael D. Gilchrist** *Laboratoire LM3, ENSAM Paris **Department of Mechanical Engineering, NUI Dublin Micromechanical approach

2
A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State SOLUTIONS: 1.Phenomenological behaviour law identification under specific loading. What happens if : Loading changes (strain rate effects ?) Reinforcement change (shape, nature, volume faction, etc.) ? Time consuming, expensive PROBLEM: Knowing the mechanical response of a reinforced polymer under a given loading when the matrix is nonlinear viscoelastic

3
PROBLEM: Knowing the mechanical response of a reinforced polymer under a given loading when the matrix is nonlinear viscoelastic SOLUTIONS: A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State 2.Building a theoretical model which accounts for : Different loading cases Different reinforcement situations (nature, shape, volume fraction, etc.) Based on : Knowledge of each reinforcement behaviour Knowledge of the microstructure HOMOGENISATION APPROACH

4
OUTLINE 1. Homogenisation basics 3. Theoretical model 2. Constituents behaviour 4. Model theoretical predictions 5. Conclusion A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

5
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State 3 BASIC STEPS: 1. Description Elastic, plastic, viscoelastic, nonlinear, etc. Behaviour law identification of each constituent Description of the microstructure Shape of the reinforcements Orientation of the reinforcements Volume fraction of the reinforcements Position of the reinforcements

6
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State 3 BASIC STEPS: 2. Localisation: Reinforcement (phase 1) Matrix (phase 0) What are the stresses and strains in each of the constituent phases when a macroscopic loading is applied ? Solution of a structure problem Functions of the description and the homogenisation scheme (hypothesis on which the solution is based)

7
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State 3 BASIC STEPS: 3. Homogenisation:How to relate the loading in each phase to the macroscopic loading ? Transition from the micro scale to the macro scale Equilibrium Behaviour Localisation

8
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State Material studied Glass bead reinforced polypropylene (10% to 30 %) Beads assumed to be randomly distributed Glass assumed to be linear elastic Polypropylene assumed to obey a Schapery type behaviour law

9
Schapery type behaviour law: Linear viscoelastic creep compliance Time-shift factor Generalised stress Elastic part Viscoelastic part BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

10
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State MODEL ELABORATION: Homogenisation schemes well established for linear elastic materials What happens if : One constituent is linear viscoelastic ? Nonlinear (elastic, plastic) ? Nonlinear viscoelastic ? +

11
Homogenisation for linear viscoelastic materials: Linear viscoelastic behaviour law Laplace – Carson transform Analogy with linear elastic behaviour Homogenisation carried out in the Laplace – Carson space Time domain solution obtained by inverse transform of the symbolic solution BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

12
Thermoelastic problem Homogenisation for nonlinear materials: Non-zero initial loading Tangent modulus calculated for a given loading 0000 Linearisation Affine formulation BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

13
Homogenisation for nonlinear viscoelastic materials: Linearisation of the nonlinear viscoelastic material into a linear viscoelastic material 1. 2. Solve the homogenisation problem with the Laplace – Carson transforms Suggested linearisation : Tangency in t n for the same load history Stress free deformation history BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

14
Homogenisation for nonlinear viscoelastic materials: Linearisation example Tensile loading at constant STRESS rate BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

15
Homogenisation for nonlinear viscoelastic materials: BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State LinearisationLaplace – Carson transform Matrix behaviour Glass behaviour Reinforcements shape and orientation Reinforcements volume fraction Localisation as per the Mori – Tanaka scheme in the Laplace space Homogenisation Inverse Laplace Carson Transform Macroscopic response of the whole composite

16
Simulated response to a uniaxial stress load applied at a stress rate of 5 MPa / sec for various volume fractions of glass beads reinforced polypropylene BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

17
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State Effect on the strain at 25 MPa of the stress rate for simulated uniaxial loadings at a constant stress rate for various volume fractions of reinforcements

18
BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State CONCLUSION Theoretical model taking into account the nonlinear viscoelasticity Matrix behaviour Reinforcements behaviour Reinforcements shape and orientation Reinforcements volume fraction Global composite behaviour

19
Identification of a Schapery type behaviour law: 2 1 11 Creep - recovery tests where 11 and 22 are sufficient to identify the full 3D behaviour law t t BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

20
Identification of a Schapery type behaviour law: If the behaviour is linear viscoelastic Evaluated for a low level of stress t Evaluated by nonlinear regression Evaluated with the transverse data BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

21
Identification of a Schapery type behaviour law: Some results: Prony series BASICS MODEL PREDICTION CONCLUSION BEHAVIOUR A Micromechanical Model for Non-Linear Viscoelastic Particle Reinforced Polymeric Composite Materials – Undamaged State

Similar presentations

OK

COMING FROM? IMDEA Materials Institute (GETAFE) Polytechnic University of Madrid Vicente Herrera Solaz 1 Javier Segurado 1,2 Javier Llorca 1,2 1 Politechnic.

COMING FROM? IMDEA Materials Institute (GETAFE) Polytechnic University of Madrid Vicente Herrera Solaz 1 Javier Segurado 1,2 Javier Llorca 1,2 1 Politechnic.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on nutrition in plants and animals Ppt on beer lambert law spectrophotometry How to save ppt on ipad mini Ppt on game theory youtube Ppt on 2nd world war pictures Ppt on case study of apple Ppt on cse related topics Ppt on deccan plateau of india Ppt on family planning in india Ppt on 98 notified sections of companies act 2013